Int. J. Hydrogen Energy, Vol. 9, No. 3, pp. 215-218, 1984. Printed in Great Britain.
0360-3199/84 $3.00 + 0.00 Pergamon Press Ltd. © 1984 International Association for Hydrogen Energy.
ELECTROCHEMISTRY OF FUEL CELLS FOR TRANSPORTATION APPLICATIONS E. R. GONZALEZand S. SRXNIVASAN Los Alamos National Laboratory, P.O. Box 1663, Los Alamos, NM 87545, U.S.A.
(Received 9 February 1983) Abstract--Fuel cells are promising power sources for electric vehicles and do not suffer from the inherent limitations of efficiency, energy density, and lifetime, as encountered with all types of batteries considered for this application. The projected performance of fuel-cell vehicles is comparable to that of the internal combustion and diesel engine vehicles but with the additional advantages of higher fuel efficiency, particularly with synfuels from coal. The ideal fuel for a fuel-cell power plant for electric vehicles is methanol. This fuel is reformed to hydrogen, which combines with oxygen from the air in an acid electrolyte (phosphoric, solid polymer, or superacid) fuel cell to produce electricity. Though the phosphoric acid fuel cell is in the most advanced state of development (mainly for power generation applications), the solid polymer and superacid electrolyte fuel cells are more promising for the transportation application because of the faster oxygen reduction kinetics (and hence potential for higher power densities) and shorter start-up times. Alkaline electrolyte fuel cells can be used only with pure hydrogen (which causes a weight or energy penalty for any of the methods it can be carried on board the vehicle), but have the best potential for minimizingor eliminating noble metal requirements. The paper summarizes needed areas of research (i.e. reduction or elimination of noble metal loading, finding CO-tolerant electrocatalysts, finding less expensive solid polymer electrolytes, synthesis and elucidation of higher molecular weight superacids) to advance fuel-cell technology for vehicular applications.
R A T I O N A L E AND E L E C T R O C H E M I C A L REQUIREMENTS The energy crisis after the oil embargo in 1973 stimulated research and development in power plants for electric vehicles. Vehicles with batteries face serious problems such as the need for long periods of recharging, low energy density, and poor cycle life. In the 1970s, concentrated efforts were made to develop advanced batteries with performance characteristics superior to those of lead-acid batteries. Though many of these battery systems showed promise initially, the R&D programs demonstrated difficulties in overcoming the above problems. If electric vehicles are to approach the performance characteristics of diesel-engine and internal-combustion-powered vehicles in respect to range and acceleration but with more efficient fuel utilization, the most promising source appears to be a fuel cell using reformed methanol. In order to advance fuel-cell technology for vehicular applications, several electrochemical considerations are essential. This paper focuses on these aspects in an analysis of the potential fuel-cell systems as power sources for electric vehicles. In establishing the needs in terms of performance of fuel cells for transportation, the first parameter that has to be defined is the type of fuel. One of the most promising fuels is methanol , which can be obtained from coal, natural gas, or biomass, and can easily be converted to H2 in a reformer. It is possible that in the future, an abundance of H2 fuel will be produced
transport, and handle this fuel will have to be devised. From the computer simulation studies of Lynn , it is possible to list the electrochemical requirements of fuel cells for transportation, and these are presented in Table 1. Parameters such as the current density, cell potential, noble metal loading, and internal resistance are related to the kinetics of the electrode processes and the conductivity of the electrolyte. Also, the performance and the life of the cell are dependent on the extent of CO chemisorption on the electrocatalyst particles, the sintering of these particles, and electrochemical corrosion of the support materials. Table 2 shows the main characteristics of the promising types of fuel cells for electric vehicles. The elec-
Table 1. Background--essentialelectrochemicalrequirements of fuel cells for electric vehicles
because of the development of nuclear and fusion reactors. However, efficient and safe ways to store, 215
High power density (> 130 mW/cm2) High efficiency (> 30%) Low oxygen overpotential (< 400 mV) Fast start-up time (< 5 min) Fast response to transients Lifetime of 5000--6000h with operation under simulated vehicle operating conditions Stability of cell component materials at close to open circuit potentials Optimize systems engineering of methanol reformer and fuel cell Reduction in noble metal loading; finding noble metal substitutes; low cost of other cell components Minimal poisoning of anode by impurities
E.R. GONZALEZ AND S. SRINIVASAN Table 2. Promising types of fuel cells for electric vehicles Fuel
Operating temperature (°C)
Methanol Methanol Methanol
83-100%H3PO4 Nation Superacids-TFMSA, higher homologs 25-50% KOH
150-225 80-150 60-150
Pt; intermetallics Pt; intermetallics Pt; intermetallics
trochemistry of each of these systems will be presented in the following sections,
Pt; intermetallics; and non-noble metals, e.g. Ag with and without additives
complexes show good performance  at temperatures up to 120°C but are unstable in the phosphoric acid environment above this temperature.
Phosphoric acid electrolyte fuel cell The phosphoric acid fuel cell (PAFC) is in the most advanced state of development and its potential for vehicular application is currently under investigation at Los Alamos. The cell needs a relatively high temperature of operation ( - 200°C) to overcome the low conductivity of the electrolyte and the slow kinetics of the oxygen reduction reaction. Recently, a study  of the interracial characteristics between mercury electrodes and 95% phosphoric acid was carried out using thiourea as a probe species, The results showed that the double layer is thicker in phosphoric acid (6/~) than in aqueous media (4 A). This means that the electron transfer during oxygen reduction at the electrode-phosphoric acid interface occurs over a wider barrier than at an electrode-aqueous electrolyte interface and hence can be expected to be considerably slower in the former case. Also, it was found that H3PO4 is more strongly adsorbed than water, Thus, the adsorption of reactants and intermediates, which leads to faster reaction rates, will be more difficult in concentrated phosphoric acid than in aqueous electrolytes. This is confirmed by the experimental results that the oxygen reduction kinetics is two orders of magnitude faster in dilute HaPO4 than in the concentrated acid . In the phosphoric acid fuel cell, the electrocatalyst consists of platinum particles on a conducting carbon substrate. The platinum can be poisoned by chemisorption of CO, an impurity ( - 1%) present in reformate fuels. At temperatures exceeding 180°C, this effect is not too serious, and about 1% CO can be tolerated. It has also been observed that the Pt particles tend to sinter via an electrocrystallization process  with the consequent loss of active area. A third problem presented by the electrocatalyst is the loss of platinum on the electrolyte side. This could be related to corrosion processes of the platinum and of the carbon support when close to the open circuit potentials. This shows the need for electrochemical research oriented toward finding suitable substitutes for noble metal electrocatalysts and carbon supports. Some metal-organic
Solid polymer electrolyte fuel cell At present solid polymer electrolyte fuel cells use Nation as the electrolyte . This membrane is quite expensive; it is predicted to have a lifetime in fuel cells (100000 h) that far exceeds the needs for transportation applications (5000 h). Enhanced oxygen reduction kinetics on platinum in this medium and low internal resistances make it possible to achieve higher power densities than with other types of fuel cells. Further electrochemical research, systems design, and engineering are still needed prior to the development of power plants for vehicular applications. The main problem with this type of cell has been water management when operated above 100°C because the drying out of Nation makes it nonconducting. Several methods are being explored to keep the membrane wet. The present platinum loading is about ten times higher than that for the phosphoric acid fuel cell. However, power densities in the solid polymer electrolyte fuel cells are about three times higher than the phosphoric acid fuel cell. Efforts to lower noble metal loadings by use of supported electrocatalysts are still necessary. Because of the water management problem, solid polymer electrolyte fuel cells along with alkaline and superacid electrolyte fuel cells are restricted to the low temperature of operation (< 100°C), which means a faster start-up time, a very important factor in transportation applications. On the other hand, the problem of CO chemisorption at these temperatures may be enhanced, which again points to the need for more electrochemical research leading to electrocatalysts that are tolerant to CO.
Superacid electrolyte fuel cells At present, the onlysuperacidcommericallyavailable is trifluoromethanesulfonic acid (CFaSO3H, commonly referred to as TFMSA). Interest in this acid is based on the fact that the oxygen reduction reaction in aqueous TFMSA is much faster than in concentrated phosphoric acid [8, 9]. As discussed above, this can be explained
ELECTROCHEMISTRY OF FUEL CELLS
Table 3. Needed areas of electrochemical research on fuel cells for electric vehicles Phosphoric acid fuel cells: improvements in oxygen reduction kinetics evaluation of performance of cell under simulated vehicle operating conditions - - reduction in noble metal loading -
Solid polymer electrolyte fuel cells: - - low cost ion exchange membrane - - efficient water management to allow operation above 100°C --reduction in noble metal loading Superacid fuel cells: selection and synthesis of higher molecular weight acids acid concentration management with TFMSA substitutes for noble metals -
Alkaline fuel cells: efficient CO2 removal membrane for operation with reformed methanol lower internal resistance of cell substitutes for noble metals -
partly by a reduced thickness of the double layer in the aqueous medium. Recently, the double layer properties of mercury electrodes in solutions containing CF3SO3 anions were investigated . It was concluded that CF3SO~ adsorbs very weakly on electrodes and even desorbs at sufficiently anodic potentials. Thus, the presence of these anions in the electrolyte should not interfere with the adsorption of reactants or intermediates for the oxygen reduction reaction. Early work with TFMSA involved the use of the monohydrate in systems similar to those using phosphoric acid. Because the monohydrate wets Teflon, research on this acid as the electrolyte was steered in the direction of aqueous solutions . TFMSA has a relatively high vapor pressure. Consequently, efforts are being focused on the synthesis of higher homologs such as tetrafluorethanedisulfonic acid . This acid does not wet Teflon so readily because of a higher sulfonic group/fluorine atom ratio, Because of the enhanced oxygen reduction kinetics in these superacids, it is expected that fuel-cell power densities will be twice as high as those obtained in PAFCs. This means that there is room for electrochemical research toward reducing the noble metal loading or the use of nonnoble metal catalysts,
Alkaline electrolyte fuel cell The alkaline electrolyte was the first to be developed, but progress has not been too evident because of the stringent limitation imposed that the inlet gases must not contain even trace amounts of CO2. The electrochemistry of these cells is highly satisfactory because at relatively low temperatures (< 100°C) the oxygen reduction kinetics even with nonnoble metal catalysts (e.g.) is sufficiently fast [13, 14]. These cells need to operate with a circulating electrolyte. Because of this, the internal resistance of the cell tends to be relatively
high, making it difficult to attain high current densities. Thus, for transportation applications the power output from cells for start-up and acceleration is very limited requiring hybrid configurations involving secondary batteries. These problems could certainly be overcome, but the development of the alkaline electrolyte fuel cells is tied to the availability of pure H2 as well as to the advancement of ways of storing and handling this fuel. CONCLUSIONS Electrochemical considerations are essential in determining the suitability of particular fuel-cell systems for transportation applications. Fundamental research is needed on all four types of fuel cells in areas such as the effects of electrode materials and electrolyte composition on the oxygen reduction kinetics, electrosorption of CO on noble metals and alloys, electrocrystallization processes leading to the sintering of catalyst particles, and the development of nonnoble metal catalysts. Needed areas of research are listed for each type of fuel cell in Table 3. At the same time, it must be kept in mind that the performance and lifetime of a fuel-cell system are dependent on the operational characteristics. Until the present time, most studies have been carried out under continuous operation at nearly constant power levels for power generation applications. For this reason, investigations are under way at Los Alamos National Laboratory to examine the variation of performance of fuel cells when subjected to simulated drive cycles and to elucidate the mechanism of performance degradation under such conditions.
Acknowledgements--This work was performed under the auspicesof the U.S. Department of Energy. Dr E. R. Gonzalez would like to thank CNPq, Brazil, for a scholarship during his sabbatical leave from the Instituto de Fisica e Quimica de Sfto Carlos.
E . R . GONZALEZ AND S. SRINIVASAN
7. J. F. McElroy, Proceedings of the 28th Power Sources Symposium, Atlantic City, New Jersey, June (1978). 1. B. McCormick, J. Huff, S. Srinivasan and R. Bobbett, 8. J. Appleby and B. S. Baker, J. Electrochem. Soc. 125,404 Applications scenario for fuel cells in transportation, Los (1978). Alamos Scientific Laboratory Report LA-UR-7634-MS 9. S. Srinivasan and H. Olender, Fuel Cells: applied research (1979). - - electrocatalysis and materials, Annual Report for 1976, 2. D. Lynn, Analysis of vehicle systems using hydrogen Brookhaven National Laboratory BNL 50652 (1977). storage/alkaline fuel cell technology. Los Alamos 10. E. R. Gonzalez, K.-L. Hsueh and S. Srinivasan, ElectroNational Laboratory unpublished report, LA-UR-80-3094 chim. Acta 27, 1425 (1982). (1980). 11. M. A. George, Abstracts of the National Fuel Cell Seminar, 3. E. R. Gonzalez, K.-L. Hsueh and S. Srinivasan, J, Elecp. 123. San Diego, California, July (1980). trochem. Soc. 129, 1 (1983). 12. M. A. Walsh, J. Eynon and R. S. Morris, Abstracts of the 4. K.-L. Hsueh, E. R. Gonzalez and S. Srinivasan, Extended National Fuel Cell Seminar, p. 86. Norfolk, Virginia, June Abstracts of the 161st Meeting of the Electrochemical (1981). Society, Vol. 82-1, p. 1080. Montreal, Canada (1982). 13. K. Mund, G. Richter and F. von Sturm, Proceedings of 5. K. Kinoshita, Proceedings of the Workshop on the Electhe Workshop on the Electrocatalysis of Fuel Cell Reactions trocatalysis of Fuel Cell Reactions (W. E. O'Grady, S. (W. E. O'Grady, S. Srinivasan and R. F. Dudley, eds.), Srinivasan and R. F. Dudley, eds.), Vol. 79-2, pp. 144Vol. 79-2, 47-66, The Electrochemical Society, Princeton, 164. The Electrochemical Society, Princeton, New Jersey New Jersey (1979). (1979). 14. J. McBreen, G. Kissel, F. Kulesa, E. Gannon, S. Srini6. M. Walsh, D. N. Crouse and F. Walsh, Abstracts of the vasan and K. R. Kordesch, 15th Intersociety Energy ConNational Fuel Cell Seminar, p. 115. Bethesda, Maryland, version Engineering Conference, Seattle, Washington, June (1979). Paper No. 809174, August (1980). REFERENCES